Abstract
Organic electronics offers prospects of functionality for science, industry and medicine that are new as compared with silicon technology and available at a very low material cost. Among the plethora of organic molecules available for materials design, polymers and oligomers are very promising, for example, because of their mechanical flexibility. They consist of repeated basic units, such as benzene rings, and the number of these units N determines their excitation gap, a property that is often used in proposals of organic photovoltaics. Here, we show that contrary to a widely held belief the magnitudes of excitation gaps do not always decay monotonously with N, but can oscillate due to the presence of a ‘Dirac cone’ in the band structure. With an eye on the more fundamental question how a molecular wire becomes metallic with increasing length, our research suggests that the process can exhibit incommensurate oscillations.
Introduction
Oligoacenes are molecules that consist of fused benzene rings (Fig. 1a). The shortest examples—benzene, naphthalene and anthracene—are of fundamental importance in chemistry. While the synthesis of gasphase oligoacenes with more than six rings (hexacene) remains a challenge^{1}, there are reports that attempts are on the way for onsubstrate synthesis^{2}. On the theory side, oligoacenes have been subject of an intensive debate due to pronounced correlation effects^{3,4}. Much of the interest in this class of molecules is driven by organic electronics^{5} and photovoltaics^{6,7}, where oligoacenes and their derivatives find frequent applications^{8,9,10,11,12}. From a broader perspective, a study of systems with linearly fused rings, ‘nanographenes’, offers means to learn how properties of a molecular wire converge to the onedimensional limit.
As the number of fused molecular units increases, the optical gap either approaches a constant or vanishes. In the former case, the infinite chain is a band insulator and in the latter it is a metal. Metallic behaviour is usually manifested by a single band that crosses the Fermi energy. This band is partially filled and the gaps of chains of finite length should tend to zero as quickly as 1/N, N being the number of units.
The 1/N behaviour merely reflects the wellknown level spacing of the particleinsideabox model. Hence, the common belief that the decay is generally monotonous (possibly, with decorating evenodd oscillations). However, in this work, we demonstrate that the gap can decay in a nonmonotonous way, with strong and even incommensurate oscillations. Our calculations based on densityfunctional theory (DFT, detailed in Methods) show that the gap of the first 10 oligoacenes drops to zero quickly, but it rises up again and drops repeatedly with periodicity of 11 units (rings). By a sophisticated postDFT analysis, we clarify the conditions for observing the oscillations in oligoacenes. Remarkably, this behaviour has not been reported before in spite of the intensive research focus on these molecules. As we argue below, the gap oscillations originate from a band crossing at the Fermi level, that is reminiscent of the Dirac points and Dirac cones in certain films, such as graphene, and bulk materials. A consequence of the oscillations is that molecules with similar excitation gaps can have very different lengths. In practical terms, our research implies that the molecular length can be a parameter that can be optimized in addition to the energy gap.
Results
Singleparticle spectrum
The segmented (piecewisesmooth) form of the oligoacene gap, shown in Fig. 1b, indicates that an orbital crossing occurs at the extremal points of the gap function. We confirm this by inspecting the Kohn–Sham eigenvalue spectra in Fig. 1c. The orbital energies evolve as almost straight lines as a function of the inverse chain length and create a weblike pattern. For a given N, the highest occupied molecular orbital (HOMO) is given by the blue symbol of the highest energy; the lowest unoccupied molecular orbital (LUMO) corresponds to the red symbol of the lowest energy. Close to certain crossings, the LUMO and HOMO interchange—in this situation, the gap has a minimum. The local maxima of the gap manifest another level crossing.
Band crossing
To understand the origin of the oscillations and level crossings, we invoke the band structure of the infinite chain, ‘polyacene’, in Fig. 2. As one passes from the Γ point towards the corner of the Brillouin zone, we encounter a crossing of the valence and conduction bands at k_{D}=0.9102π/a. This peculiar band structure of polyacene wires was discussed first by Kivelson and Chapman^{13} based on an analysis of a tightbinding Hamiltonian with first (t), second (t′) and third nearest neighbour hopping (t′′). As they argued, t′′ shifts the conduction and valence bands against each other. If t and t′′ share the same sign, the shift is negative and we witness a nonavoided band crossing. From our DFTcalculation, Fig. 2, we estimate t′′=0.1t=0.31 eV by matching to the tightbinding model.
As a consequence of crossing, electrons and holes with energies sufficiently close to the Fermi level have a piecewise linear dispersion (see Fig. 2) reminiscent of the Dirac cones in graphene. Just as in graphene, the ‘Dirac point’ in polyacene is a property of the conjugated π electron system. However, in graphene, the position of the Dirac points in the Brillouin zone is dictated by the symmetry of the honeycomb lattice, while in polyacene it is controlled by t′′.
Origin of oscillations
At least in the case of sufficiently long oligoacenes, one should be able to derive their spectrum from the polyacene band structure by imposing selection rules for wave numbers due to hardwall boundary conditions (‘zonefolding’). For a given number of rings N, only selected wave numbers are allowed. We choose the following set
which applies for a guitar string of the length a(N+1), a is the length of one ring. In Supplementary Note 1, we inspect the boundary condition in detail and demonstrate in Supplementary Fig. 2 that the optimal quantization length is the one given in equation 1. Let us denote E_{g}(k) :=ε_{c}(k)−ε_{v}(k), where ε_{c,v} are the conduction and valence band energies. The optical gap will be given approximately by the energy , where denotes the wave number from the allowed set, that is closest to the Dirac point, k_{D}. Hence, labels the HOMO/LUMO pair.
As we increase the number of rings, will move and eventually cross the Dirac point, where the HOMO and LUMO interchange. This explains that the periodicity of the gap oscillations of the oligoacenes is controlled by the position of the Dirac cone in the Brillouin zone. More precisely, the period is inversely proportional to π/a−k_{D}, the distance to the zone boundary. Similarly, the maxima of the gap are also fixed by band structure consideration: it is only when the Dirac point lies in the middle between two consecutive wave numbers from the allowed set. If a local maximum occurs at N_{0} with value , its upper bound must be ℏυ_{F}π/a/(N_{0}+1), where υ_{F} is the Fermi velocity (numerically ℏυ_{F}π/a=6.485 eV).
The above considerations suggest natural energy and length scales. In Fig. 3, we show the gap expressed in these natural units (blue trace). Remarkably, our plotting exhibits a sawtooth form with well developed periodicity (with the exception of very small molecules). Furthermore, in the same plot we show —the gaps reconstructed from folding the polyacene band structure (red traces). Remarkably, both traces lie almost on top of each other. Naively, corrections of the order of 1/N to the zonefolding procedure should be expected, which means a correction of the order of 100% for benzene, N=1. In practice, the finitesize correction turns out to be much smaller. For benzene, the deviation is only 11% (tetracene 1%, hexacene 8%). We comment that the molecular gaps in Fig. 3 already involve relaxation effects that can not be accounted for in the zone folding. We see that is always higher than for N>4. We attribute this to the fact that the relaxation effects compress the length of the rings at molecule’s edges. Since the total length shrinks, the level spacing and gap increase.
We have seen that on DFT level, band structure effects control the excitation gaps of oligoacenes. It is known that the Kohn–Sham excitation gaps obtained from the DFT groundstate calculation agree with optical excitations only up to corrections that are incorporated in timedependent DFT. These corrections include a Hartree and an exchangecorrelation kernel that can renormalize the excitation energies. In ref. 14, these dynamical correction have been calculated for the smaller system sizes N=2–6 (with a hybrid functional) and turn out to be below 10% of the bare Kohn–Sham gap. As screening effects generally enhance with decreasing gap, that is, increasing system size, it is reasonable to expect that dynamical corrections do not affect the picture that we present.
Charged excitations
We now argue that the charged excitation energies, that is, the ionization energies and electron affinities, also inherit the oscillatory structure from the ‘Dirac cone’. In this section, we provide an analysis of results by DFT and various postDFT techniques. The latter can exhibit significant deviations from the DFT estimates and therefore correct for artifacts of approximate exchangecorrelation functionals^{14,15,16}.
As it is well known, in KS–DFT, the ionization potential I agrees with the HOMO energy of the chargeneutral molecule with N_{el} electrons: I=−ε_{HOMO}(N_{el}). The corresponding electron affinity A can be obtained from a reference calculation that has been performed with one additional electron: A=−ε_{HOMO}(N_{el}+1).
In contrast to DFT, in Green's function methods (such as G_{0}W_{0}), the energies of charged excitations are already incorporated in the quasiparticle (QP) energies. The G_{0}W_{0} QP band structure is shown in Supplementary Fig. 1. It shows a band pattern very similar to the DFT results. Since computational demands do not allow a fine resolution near the Fermi points, we inspect the symmetry of the four Bloch states in Fig. 4, which provides evidence of a band crossing in G_{0}W_{0}. Therefore, one expects that the charged excitations support oscillations analogous to the ones already observed in the optical gaps. The renormalized parameters of the Dirac cone are compared in Supplementary Table 1.
In what follows, we will represent the number of rings N by a dimensionless number ξ=(N+1)(1−ak_{D}/π), where k_{D} is the Dirac wave number and a is the lattice parameter. Brillouin zone folding predicts gap minima at integer ξ. The orbital energies E_{i} (i stands for HOMO or LUMO) will be represented by a dimensionless quantity .
First, we discuss the behaviour of the HOMO and LUMO (Kohn–Sham) energies on DFT–Perdew–Burke–Ernzerhof (PBE) level. The LUMO energy enters because we replace ε_{HOMO}(N_{el}+1) by ε_{LUMO}(N_{el}) thus ignoring effects of the derivative discontinuity. In Fig. 5, we show HOMO (symbols red, filled) and LUMO energies (symbols red, open), along with their counterparts from the Brillouin zone folding (solid lines). As expected, with increasing number of rings the frontier orbitals cross near ξ=1 in a linear fashion.
The frontier orbitals can be classified according to the symmetry with respect to a mirror plane that is normal to the molecular plane cutting the molecule along the long axis into two identical pieces. Notably, the energy of symmetric (antisymmetric) orbitals decreases (increases) with ξ. Hence, at ξ=1, the band theory predicts a change in the symmetry of the HOMO orbital. The reverse symmetry transitions appear at halfinteger steps in ξ. We have verified that this is indeed the case for the molecules calculated in PBE.
In the following, we explore an interesting consequence of the symmetry transition for the energies of charged excitations. To this end, we present HOMO and LUMO energies calculated in PBE0. PBE0 is a (hybrid) density functional that replaces a certain fraction λ of the PBE exchange by an exact (Hartree–Fock type) exchange. In conventional PBE0, one takes λ=25%. The derivative discontinuity, that is absent in PBE, is thus partially restored.
In Fig. 5, the (dimensionless) PBE0 energies ε_{HOMO,LUMO} are shown (green symbols). They deviate significantly from the PBE zonefolding estimates. This difference is due to λ: it vanishes continuously in the limit λ→0. The PBE0 data brings two qualitatively new features. With hybrid functionals, LUMO and HOMO energies contain a fraction of the charging energy. In PBE0, the latter is entirely given by Hartree–Fock exchange, which does not account for interaction screening. Hence, for long linear chains, the charging energy will be dominated by a spurious logarithmic length dependence. The slowly increasing deviation between the HOMO/LUMO energies and band lines for the first 10 molecules can be understood in this way. At N=11, we witness an abrupt change: a slope inversion and a step in the PBE0 trace. It can be understood in the following way. The electronic structure data for PBE0 and PBE are adiabatically connected via the λ parameter. Hence, for every system size N, the frontier energies obtained with PBE0 can be thought of as originating from a PBE reference result corrected by perturbative terms that are controlled by λ. The correction terms describe the charging energy and therefore contain Coulombmatrix elements of the PBE reference calculation. At N=11, the symmetry of the frontier orbitals of the PBE reference calculation changes. The Coulombmatrix elements react to that change and consequently the PBE0 traces exhibit a jump. In the presence of screening beyond PBE0, we expect that the spurious logarithm disappears in the limit ξ→∞ and the step will be weaker.
The G_{0}W_{0} QP energies are also shown in Fig. 5. It is easy to understand the differences between all methods presented if we recall that the PBE0 values contain a fraction of the charging energy, while the G_{0}W_{0} values fully include charging effects. Consequently, for benzene, the difference in orbital energies is approximately four times the difference and the same holds true for LUMO. We notice that for longer molecules, the relative difference drops below four, because of the screening mechanism in G_{0}W_{0} that is absent in PBE0. Due to high computational demands, we could not obtain QP energies for systems beyond N>4 rings.
Correlation effects
To rigorously establish the validity or our conclusions even in the presence of strong correlations (where ab initio methods tend to fail), we analyse a (parameterized) model system, the oligoacene Hubbard model. We solve it numerically at different values of the interaction strength by employing the densitymatrix renormalization group (DMRG), see Methods for details. We first discuss a model with spinless fermions. Results for the optical gap are show in Fig. 6 for various values of N and nearest neighbour interaction U_{1}. As we see, the N oscillations of the optical gap survive even up to interactions comparable in strength with the bandwidth. The period can be renormalized to the extent that for large interaction the oscillation period increases. At a certain critical value comparable to the bandwidth, U_{1}≈5 eV, the period diverges. At large interactions U_{1}>>5 eV, we find a (twofold degenerate) nearest neighbour charge density wave ground state.
Our DMRG results for the spinfull calculation at low interaction strength are depicted in Fig. 7a. The data confirms that the oscillation phenomenon is stable against the presence of weak interactions. Figure 7b displays the dependency of the optical gap on the onsite interaction, U_{0}. Three molecules are shown with a length N that is close to the optimal length N_{min}≈10 where the gap is expected to exhibit particularly small excitation gap. In the perturbative regime U_{0}≪2t, switching on U_{0} even stabilizes the oscillations and makes them more pronounced in the sense that the ratio between the minimal gap near N_{min}≈10 and the neighbouring gaps goes through a maximum at finite U_{0}. At interaction strength U_{0}≲2t, the excitation energy for N=10 is significantly smaller than for the neighbouring molecules N=9,11. Only at U_{0}≈6 eV, the two traces (N=9,10) cross. At larger values, a monotonous order (in N) of the traces is established.
By performing an independent DMRG calculation in the spinsector S=1, we have checked that the optical gap coincides with the spin gap for the values of U considered in this manuscript.
The scaling of the excitation gap with system size is shown in Fig. 8. For smaller molecules, an approximately exponential decay is observed that can be fitted by
with Δ_{0}≈7.8 eV and N*≈2.3. Since the quasiexponential decay is already seen at weak interactions including U_{0}=0, it is unrelated to correlation effects, such as ground state magnetism. Interaction effects become relevant only at N≳N* and very strong values of U_{0} that significantly exceed the bandwidth ≈2t. In this regime, the gap oscillations disappear and a monotonous behaviour sets in, see Fig. 8
Discussion
Over the years, there has been intensive theoretical and experimental work that addresses the nature of the groundstate of oligoacenes, for review, see refs 1, 4. The topic of interest is whether the ground state could be magnetic (open shell, radical) or at least close to a magnetic (or other) instability. We discuss a selection of earlier work that appears most relevant to us in the light of our new findings.
In DFT studies employing hybrid functionals, brokensymmetry, spinpolarized ground states have been reported^{17}. Since approximate functionals underestimate quantum fluctuations, they tend to overestimate the tendency for symmetry breaking. Therefore, such studies are difficult to interpret. Indeed, our DMRG calculations indicate that the ground state does not exhibit a (simple) brokensymmetry phase. To be consistent with this finding, we employ in our DFT studies nonmagnetic, closedshell calculations.
To address correlation effects, other methods have been applied. Where only relatively small system sizes could be addressed, an extrapolation of excitation energies to the polymerlimit of large N was performed (theory^{3} N≤12, experiment^{18} N≤6). For instance, Hachmann, et al.^{3} performed a DMRG study on a model of polyacene similar to ours. These authors fit their data for the spintriplet gap in the manner ΔE_{st}≈Δ_{st}+δ_{st} exp(−N/N_{st}) with a nonvanishing offset Δ_{st}≈0.144±0.017 eV (orig: 3.33±0.39 kcal mol^{−1}). The offset indicates the presence of strong correlations that have been interpreted as a singlet ground state with an open shell (di or polyradical). A finite offset has also been reported in another DMRG study on an oligoacenelike Heisenberg model (up to N=28)^{19}. Since the Heisenberg Hamiltonian ignores charge fluctuations, the latter result carries over to oligoacenes only in the Mottlimit of very large U_{0}. In this regime, our results are consistent with refs 3, 19 in the sense that we confirm the absence of oscillatory behaviour, as shown in Fig. 8 for very large interaction U≳2t. In this regime, our results are also in agreement with the study of ref. 20 where in the large U limit an enhanced ‘mottness’ for an honeycomb like twoleg ladder in comparison to a quadratic twoleg ladder was shown.
In conclusion, we show by a combination of DFT, postDFT methods (GW theory) and numerically exact Hubbardtype model calculations that oligoacenes exhibit oscillations in their fundamental excitation gaps with increasing length N. It has been shown that these oscillations result from the wellknown ‘Diractype’ dispersion of polyacene in combination with a zonefolding argument. This basic origin suggests that the effect is robust, which is an important requirement for prospective technological applications. We have seen that the oscillatory modulation of the gap dependence may be hindered if strong interactions are active. At present, a realistic estimate of the interaction strength is lacking. However, even if the Coulomb repulsion wipes out gap oscillations in the gas phase, our study suggests that these band structure effects will revive when molecules are embedded in screening environments, such as electrochemical solutions^{21} or synthesized on surfaces, where the effective screened interaction will be several times reduced as compared with the gasphase value.
Methods
Densityfunctional calculations
We employ the usual Kohn–Sham densityfunctional method^{22,23} implemented in the FhiAims package^{24}. The optical gaps were calculated using the Perdew–Burke–Ernzernhof^{25} functional. The spinrestricted (closed shell) Kohn–Sham equations were solved in a nonrelativistic form, with relativity included a posteriori by rescaling the Hamiltonian eigenlevels, according to the zeroth order regular approximation^{26}. The basis set for hydrogen (carbon) contained totally 15 (39) functions of angular momenta up to l=4 and distinct radial dependences (the basis set is called tier2). For periodic calculation of the band structure, we sampled the Brillouin zone using 1,000 points in the reciprocal chain direction. For both periodic and nonperiodic calculations, the ground state was reached with strict convergence criteria for the difference in density (10^{−6}), total energy (10^{−7} eV) and forces (10^{−5} eV Å^{−1}). Geometries were considered optimized only after the maximum residual force dropped bellow 10^{−3} eV Å^{−1}.
The optical gap, shown in Figs 1 and 2, was approximated as the energy difference between the LUMO and the HOMO. A discussion of effects beyond this approximation is included in Results.
The G_{0}W_{0} calculations
For the QP band structure and QP spectra of finite chains, we have used Vienna Ab initio Simulation Package (VASP)^{27,28}. In VASP, the oneelectron orbitals are expressed using the projector augmented wave basis set^{29}. In this calculation, we used plane waves with 400 eV energy cutoff for the DFT starting calculation, and a cutoff of 300 eV for the response functions. First, standard Kohn–Sham DFT calculations were performed, using the PBE^{25} exchangecorrelation functional. Then, QP corrections were included on top of the Kohn–Sham states at the nonselfconsistent, singleshot, G_{0}W_{0} level. After convergence checks, a frequency grid of 80 points and 600 bands in total was used. The QP energies were represented on a mesh of 11 kpoints in the Brillouin zone.
The oligoacene Hubbard model and DMRG
Following Kivelson and Chapman^{13}, we construct a tightbinding model with a single orbital site per carbon atom at half filling and including up to third nearest neighbour hoppings t,t′ and t′′. We set t=3.1 eV, t′=0.341 eV, t′′=0.31 eV (as estimated from our ab initio band structure). We allow for onsite (U_{0}) and nearest neighbour (U_{1}) interactions, that we take as a variable parameters.
We perform an analysis based on the DMRG. DMRG is a wellestablished method suitable for studying manybody eigenvalue spectra of quasionedimensional systems with strong correlations^{30,31}. We study the oligoacene Hubbard model in a spinless and spinfull fashion. In the spinless case, we take U_{1} variable (U_{0} is meaningless). Discarded entropies during the DMRG sweeps are always below 10^{−7}, typically much lower. In the spinfull case, results are parameterized by U_{0}, while U_{1}=0. We keep up to 8,000 states per block; the dimension of the target space grows up to 4.3 × 10^{7}, the discarded entropies are considerably below 10^{−4} (even for N=21) in each DMRG step, typically significantly smaller. We employ at least seven finite lattice sweeps with an optimized infinite lattice warm up.
The optical gap is the difference between first excited and groundstate energies.
Additional information
How to cite this article: Korytár, R. et al. Signature of the Dirac cone in the properties of linear oligoacenes. Nat. Commun. 5:5000 doi: 10.1038/ncomms6000 (2014).
References
 1
Sun, Z. & Zeng, Z. Benzenoid polycyclic hydrocarbons with an openshell biradical ground state. Chem. Asian J. 8, 2873–2885 (2013).
 2
Treier, M. et al. Surfaceassisted cyclodehydrogenation provides a synthetic route towards easily processable and chemically tailored nanographenes. Nat. Chem. 3, 61–67 (2011).
 3
Hachmann, J., Dorando, J. J., Avilés, M. & Chan, G. K.L. The radical character of the acenes: a density matrix renormalization group study. J. Chem. Phys. 127, 134309 (2007).
 4
Bettinger, H. F. et al. Electronic structure of higher acenes and polyacene: The perspective developed by theoretical analyses. Pure Appl. Chem. 82, 905–915 (2010).
 5
Kuribara, K. et al. Organic transistors with high thermal stability for medical applications. Nat. Commun. 3, 723 (2012).
 6
Lipomi, D. J., Tee, B. C.K., Vosgueritchian, M. & Bao, Z. Stretchable organic solar cells. Adv. Mater. 23, 1771–1775 (2011).
 7
Dabo, I. et al. Donor and acceptor levels of organic photovoltaic compounds from _rst principles. Phys. Chem. Chem. Phys. 15, 685–695 (2013).
 8
Bundgaard, E. & Krebs, F. C. Low band gap polymers for organic photovoltaics. Sol. Energ. Mat. Sol. C 91, 954–985 (2007).
 9
Anthony, J. The larger acenes: versatile organic semiconductors. Angew. Chem. Int. Ed. 47, 452–483 (2008).
 10
Lin, C., Wang, Y.C., Hsu, S.J., Lo, C.F. & Diau, E. W.G. Preparation and spectral, electrochemical, and photovoltaic properties of acenemodified zinc porphyrins. J. Phys. Chem. C 114, 687–693 (2010).
 11
Lee, J. et al. Singlet exciton fission in a hexacene derivative. Adv. Mater. 25, 1445–1448 (2013).
 12
Wilson, M. W. B., Rao, A., Ehrler, B. & Friend, R. H. Singlet exciton fission in polycrystalline pentacene: from photophysics toward devices. Acc. Chem. Res. 46, 1330–1338 (2013).
 13
Kivelson, S. & Chapman, O. L. Polyacene and a new class of quasionedimensional conductors. Phys. Rev. B 28, 7236–7243 (1983).
 14
Malloci, G., Mulas, G., Cappellini, G. & Joblin, C. Timedependent density functional study of the electronic spectra of oligoacenes in the charge states −1, 0, +1 and +2. Chem. Phys. 340, 43 (2007).
 15
Blase, X., Attaccalite, C. & Olevano, V. Firstprinciples GW calculations for fullerenes, porphyrins, phtalocyanine, and other molecules of interest for organic photovoltaic applications. Phys. Rev. B 83, 115103 (2011).
 16
Setten, M. J. v., Weigend, F. & Evers, F. The GWmethod for quantum chemistry applications: theory and implementation. J. Chem. Theory Comput. 9, 232 (2013).
 17
Jiang, D.e. & Dai, S. Electronic ground state of higher acenes. J. Phys. Chem. A 112, 332–335 (2008).
 18
Angliker, H., Rommel, E. & Wirz, J. Electronic spectra of hexacene in solution (ground state. Triplet state. Dication and dianion). Chem. Phys. Lett. 87, 208–212 (1982).
 19
Qu, Z., Zhang, D., Liu, C. & Jiang, Y. Openshell ground state of polyacenes: a valence bond study. J. Phys. Chem. A 113, 7909–7914 (2009).
 20
Karakonstantakis, G., Liu, L., Thomale, R. & Kivelson, S. Correlations and renormalization of the electronphonon coupling in the honeycomb Hubbard ladder and superconductivity in polyacene. Phys. Rev. B 88, 224512 (2013).
 21
Capozzi, B. et al. Tunable charge transport in singlemolecule junctions via electrolytic gating. Nano Lett. 14, 1400–1404 (2014).
 22
Hohenberg, P. & Kohn, W. Inhomogeneous electron gas. Phys. Rev. 136, B864–B871 (1964).
 23
Kohn, W. & Sham, L. J. Selfconsistent equations including exchange and correlation effects. Phys. Rev. 140, A1133–A1138 (1965).
 24
Blum, V. et al. Ab initio molecular simulations with numeric atomcentered orbitals. Comput. Phys. Commun. 180, 2175–2196 (2009).
 25
Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 77, 3865 (1996).
 26
van Lenthe, E., Baerends, E. J. & Snijders, J. G. Relativistic total energy using regular approximations. J. Chem. Phys. 101, 9783–9792 (1994).
 27
Kresse, G. & Furthmüller, J. Efficient iterative schemes for ab initio totalenergy calculations using a planewave basis set. Phys. Rev. B 54, 11169 (1996).
 28
Shishkin, M. & Kresse, G. Implementation and performance of the frequencydependent GW method within the PAW framework. Phys. Rev. B 74, 035101 (2006).
 29
Blöchl, P. E. Projector augmentedwave method. Phys. Rev. B 50, 17953–17979 (1994).
 30
White, S. R. Density matrix formulation for quantum renormalization groups. Phys. Rev. Lett. 69, 2863–2866 (1992).
 31
White, S. R. Densitymatrix algorithms for quantum renormalization groups. Phys. Rev. B 48, 10345–10356 (1993).
Acknowledgements
We acknowledge the valuable discussions with S. Tretiak, O. Tal and T. Yelin. D.X. and M.A. acknowledge computational resources from HPC méso centre of Strasbourg and GENCICINES grant 2014gem1100. Part of this work was performed on the computational resource bwUniCluster funded by the Ministry of Science, Research and Arts and the Universities of the State of BadenWÃ¼rttemberg, Germany, within the framework programme bwHPC. R.K. and F.E. gratefully acknowledge the Steinbuch Centre for Computing (SCC) for providing computing time on the computer HC3 at Karlsruhe Institute of Technology (KIT) and the computing time granted by the High Performance Computing Center Stuttgart (HLRS) on the HERMIT supercomputer.
Author information
Affiliations
Contributions
R.K. performed DFT calculations; P.S. performed the DMRG study; D.X. and M.A. did the GW calculations; R.K., D.X. and M.A. performed the PBE0 calculations; R.K. and F.E. analysed the data and wrote the manuscript.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing financial interests.
Supplementary information
Supplementary Information
Supplementary Figures 12, Supplementary Table 1 and Supplementary Note 1 (PDF 87 kb)
Rights and permissions
About this article
Cite this article
Korytár, R., Xenioti, D., Schmitteckert, P. et al. Signature of the Dirac cone in the properties of linear oligoacenes. Nat Commun 5, 5000 (2014). https://doi.org/10.1038/ncomms6000
Received:
Accepted:
Published:
Further reading

Löwdin's symmetry dilemma within Green functions theory for the one‐dimensional Hubbard model
Contributions to Plasma Physics (2021)

Pushing the Limits of Acene Chemistry: The Recent Surge of Large Acenes
Chemistry – A European Journal (2021)

Dodecacene Generated on Surface: Reopening of the Energy Gap
ACS Nano (2020)

Advances and challenges in singlemolecule electron transport
Reviews of Modern Physics (2020)

Metallic bands in chevrontype polyacenes
RSC Advances (2020)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.